3D-, 2D- and 1D-supramolecular structures of {Zn[S2CN(CH2CH2OH)R]2}2 and their {Zn[S2CN(CH2CH2OH)R]2}2(4,4′-bipyridine) adducts for R = CH2CH2OH, Me or Et: polymorphism and pseudo-polymorphism
Benson, Ronald E.; Ellis, Carol A.; Lewis, Clairissa E.; Tiekink, Edward R.T.; CrystEngComm 9 (2007) 930–; doi:10.1039/b706442j

data_7202934
_publ_section_title
;
 3D-, 2D- and 1D-supramolecular structures of {Zn[S2CN(CH2CH2OH)R]2}2
 and their {Zn[S2CN(CH2CH2OH)R]2}2(4,4&#x2032;-bipyridine) adducts for
 R = CH2CH2OH, Me or Et: polymorphism and pseudo-polymorphism
;
_journal_issue                   10
_journal_name_full               CrystEngComm
_journal_page_first              930
_journal_paper_doi               10.1039/b706442j
_journal_volume                  9
_journal_year                    2007
_chemical_formula_moiety         'C17 H36 N4 O5 S8 Zn2'
_chemical_formula_sum            'C17 H36 N4 O5 S8 Zn2'
_chemical_formula_weight         763.84
_chemical_name_systematic
;
?
;
_space_group_IT_number           2
_symmetry_cell_setting           triclinic
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                95.483(13)
_cell_angle_beta                 96.282(10)
_cell_angle_gamma                100.576(11)
_cell_formula_units_Z            2
_cell_length_a                   10.470(4)
_cell_length_b                   12.345(6)
_cell_length_c                   12.615(6)
_cell_measurement_reflns_used    1913
_cell_measurement_temperature    173(2)
_cell_measurement_theta_max      30.3
_cell_measurement_theta_min      2.4
_cell_volume                     1582.0(12)
_computing_cell_refinement       CrystalClear
_computing_data_collection       'CrystalClear (Rigaku, 2005)'
_computing_data_reduction        CrystalClear
_computing_molecular_graphics
'ORTEPII (Johnson, 1976) & DIAMOND (Crystal Impact, 2006)'
_computing_publication_material  SHELXL97
_computing_structure_refinement  'SHELXL97 (Sheldrick, 1997)'
_computing_structure_solution    'PATTY in DIRDIF92 (Beurskens et al., 1992)'
_diffrn_ambient_temperature      173(2)
_diffrn_measured_fraction_theta_full 0.958
_diffrn_measured_fraction_theta_max 0.958
_diffrn_measurement_device_type  AFC12\K/SATURN724
_diffrn_measurement_method       \w
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71070
_diffrn_reflns_av_R_equivalents  0.068
_diffrn_reflns_av_sigmaI/netI    0.079
_diffrn_reflns_limit_h_max       12
_diffrn_reflns_limit_h_min       -12
_diffrn_reflns_limit_k_max       15
_diffrn_reflns_limit_k_min       -15
_diffrn_reflns_limit_l_max       15
_diffrn_reflns_limit_l_min       -15
_diffrn_reflns_number            14760
_diffrn_reflns_theta_full        26.0
_diffrn_reflns_theta_max         26.0
_diffrn_reflns_theta_min         2.4
_diffrn_standards_decay_%        '< 1'
_diffrn_standards_interval_count 0
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    2.078
_exptl_absorpt_correction_T_max  1
_exptl_absorpt_correction_T_min  0.858
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'ABSCOR (Higashi, 1995)'
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    1.603
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       needle
_exptl_crystal_F_000             788
_exptl_crystal_size_max          0.31
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.03
_refine_diff_density_max         0.59
_refine_diff_density_min         -0.74
_refine_diff_density_rms         0.113
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.14
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     345
_refine_ls_number_reflns         5958
_refine_ls_number_restraints     5
_refine_ls_restrained_S_all      1.14
_refine_ls_R_factor_all          0.087
_refine_ls_R_factor_gt           0.069
_refine_ls_shift/su_max          <0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0523P)^2^+2.0169P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.151
_refine_ls_wR_factor_ref         0.163
_reflns_number_gt                4784
_reflns_number_total             5958
_reflns_threshold_expression     I>2\s(I)
_cod_data_source_file            b706442j.txt
_cod_data_source_block           (3)
_cod_original_cell_volume        1581.9(12)
_cod_original_sg_symbol_Hall     '-P 1 '
_cod_database_code               7202934